Weldability Investigation and Optimization of Process Variables for TIG-Welded Aluminium Alloy (AA 8006)

Department of Mechanical Engineering, Saveetha School of Engineering, SIMATS, Chennai 602105, Tamil Nadu, India Department of Mechanical Engineering, Chendhuran Polytechnic College, Pudukkottai 622507, Tamil Nadu, India Centre for Materials Engineering and Regenerative Medicine, Bharath Institute of Higher Education and Research, Chennai 600073, Tamil Nadu, India Department of Mechanical Engineering, C. Abdul Hakeem College of Engineering & Technology, Vellore 632509, Tamil Nadu, India Department of Electrical and Electronics Engineering, KPR Institute of Engineering and Technology, Coimbatore 641407, Tamil Nadu, India Department of Mechanical Engineering, K. Ramakrishnan College of Engineering, Trichy 621112, Tamil Nadu, India Department of Mechanical Engineering, Faculty of Manufacturing, Institute of Technology, Hawassa University, Hawassa, Ethiopia


Introduction
In recent trends, aluminium alloys have been broadly applied in various work fields, being simple in construction, carriage, and marine and advanced aerospace application like wing sections, etc. Its magnificent performance will be used to fabricate lightweight containers in sheet metal work. Typically aluminum alloys are in the same light time; they will be of high strength and flexible nature. e combination of good corrosion resistance and excellent wear resistance is possessed in aluminium alloys. e permanent and rigid joining of aluminum alloy was carried out through the welding process; in the normal welding process, aluminum alloy's consolidation is challenging. Nowadays, aluminium alloys are welded simply using TIG welding for various thicknesses of the specimen. Comparatively the TIG welding process yields high quality welding joints (lesser defects), easy and faster than arc welding. Microstructural grains strength is improved in the TIG welding process, and it is noted in the mechanical strength analysis. High-quality welding was obtained compared to another welding process. It is an added advantage in the TIG welding process.
Aluminum has a mixture of properties quite difficult to find in our world: lightweight, very strong, very malleable, and nonreactive. It is the lightest metal on Earth, exceptionally bendable and rustproof due to a thin layer of chromium on its surface and is equally powerful. It does not magnetize all types of metal (except for some less-ferromagnetic metals), rendering it ineffective as a fantastic conductor of electricity [1]. Friction welding, also because the weldment generates low heat, means that residual stresses are kept low. A transverse force in wench (also known as transverse or transverse frictional force) is employed in stress measurement [2] Dengkui et al. [3] revealed that the material's mechanical properties are changed by applications of different geometric shapes. e authors studied and reported that weld joints characterization such as weld width, penetration depth, and the reinforcement process profiles could achieve it. e mechanical properties were altered, and enhanced strength was also obtained. From this study, the WZ and PMZ hardness values were decreased and weaken the joints and mechanical properties. Aravind and Daniel Das [4] suggested that the maximum welding strength attained using the process parameters (current, welding speed, and welding time) achieving the optimum tensile strength is 130. 27 MPa. e S/N ratio also states that to ensure the maximum weld strength. Ramandeep et al. [5] revealed the welding current raised the hardness of the weld joint. For their study, the welded specimens' properties are affected by the welding defects like porosity, which reduces its tensile strength. Gurmeet et al. [6] analyzed experimental comparison of TIG welding and FSW process to understand the metallurgical properties of the base material and welded area. Further their study found the hardness of the TIG welding joint and compared it to other welding joints. Lakshman et al. [7] suggested that the TIG-welded aluminium alloy offered maximum tensile strength by influencing optimum process parameters such as welding speed, gas flow rate, and welding current. In this study, they recommended better results in the post-heat-treatment process, even using different materials. Ji-Kun et al. [8] performed the TIG welding of aluminium alloy 2219. It proved the enhanced properties of hardness and tensile occurring in the postweld heat-treatment process. ey also concluded that the higher elongation and impact toughness could be obtained by implementing postweld heat treatment. Temmar et al. [9] stated the AA7075 welded joints' tensile strength was increased by applying postweld aging behavior. In the AA7075-welded joints, the significant effect decreases the impact energy.
Adalarasan et al. [10] reported that the aluminium alloy 6061 has to be welded by the TIG welding process, the optimal process parameters as 24 V, 180 Amps, 110 mm/min welding speed, and gas flow at the rate of 12 l/min. ey also evaluated the significant contribution of welding current through ANOVA and considered the primary controllable parameter. Sethuraman et al. [11] studied the optimization parameters of peak current (130, 150, and 170 Amps), base voltage (20,25,30 Amps), and gas pressure (4, 5, 6 kg/cm 2 ) of TIG welding on AA6063. e effect of each individual parameter was found, which is the most appropriate one with the help of ANOVA and regression analysis. Shanavas et al. [12] made analysis to obtain the most suitable parameters such as 180 Amps, 100 mm/min welding speed, and inert gas float 11 l/m. ey also concluded the superior tensile strength was obtained more than other joints. With the best of the search, the weldability studies in the TIG method for Aluminum AA8006 alloy were not reported in the literature. Joints have become much more prone to fatigue, making the aluminum 2219 more difficult to weld than originally thought. Researchers have developed a number of mechanisms to try to handle these constraints that incorporate AC TIG (addressing everything soldering), VPT (validating every parameter), and plasma solutions to develop VPT (resolving all the problems of curability). Nonetheless, there has been no solution to the instability/ inconsistency and the cycle of the welding procedure for the AC technique, to the point where it is no longer an issue. In order to use the variable polarity plasma soldering device, a solder joint must be created that is successful. High-perforge layers must be used for the job of soldering large sheets of aluminum, and a large amount of heat is required. Despite being smaller than usual for an AC TIG process, the current used is still high [13][14][15][16]. For AA6061 and AA7075, a comparison of TIG and FSW residual stresses revealed that the longitudinal residual stress is greater than the traverse residual stress in the welded joint [17]. e comparative investigations in terms of heat transfer and residual stress were not properly analyzed in the literature. e residual stresses and heat transfer affect the welding quality at the beginning and end of the joints. In thin plate welding, in analyzed cases it was found that the increase of spindle rotation in friction stir welding increases the tensile strength on joints initially and it declines after certain extent. e microhardness of the welded joint was measured by three layers (i.e., the top, middle, and bottom). e upper layer of bonding has a higher degree of recrystallization and dynamic recovery. e lower layer under the mechanical action of the tool pin is strongly agitated so that each layer of the sold joint has the various mechanical properties [18]. e AA2024 was successfully applied with a new welding approach by TIG β FSP to improve the mechanical properties of the TIG-welded joints. ey find that TIG welding joint defects and porosities are fully reduced by the FSP method and the microstructure and mechanical properties of the welded joint were increased by using of FSP; it has been altered [19] effectively. Using the FSP on the TIG-welded joint, the ductility and the tensile strength of the welding joint AA5083-H112 FSP and TIG were improved [20]. e present study was focused on the improvement of mechanical properties and the residual stress distribution on the welding of aluminum AA8006 alloy in the TIG welding method and optimizing process parameters for obtaining quality weld. 2 Advances in Materials Science and Engineering

Material.
In this work, a commercially available aluminium alloy 8006 plate is purchased with the required dimensional plate form characters. Before welding, the bulky AA8006 plate is further cut into 150 × 50 × 3 mm by way of wire-cut EDM. Additionally, it can be finished by a grinding and polishing process [21]. In this study, aluminum alloy 8000 series are taken to investigate the mechanical properties. AA8006 is termed as the wrought alloy. is type of alloy, generally having excellent corrosion prediction nature and having enhanced resistance, also possesses high strength [22]. It is available in foil nature due to its high strength and superior formability. It can be used in the food packing industries, medical equipment manufacturing industries, etc. is investigation used 3 mm thick AA8006 aluminium alloy plates for experimentation. Tables 1 and 2 present the chemical composition and mechanical properties of AA8006, respectively.

Taguchi's Design for Experimentation.
Usually aluminium alloy welding joints experiments are carried out as per Taguchi method, because Taguchi technique reduces the number of trials and gives optimum results with minimum time and cost [23][24][25][26]. e Design of Experiments (DOE) studied by Taguchi by way of orthogonal arrays (OA) is to improve the process parameters affecting the process with different levels [27]. In this examining L 9 orthogonal array is preferred to play the experimentation and optimize the parameters. Typically, the orthogonal array (OA) degrees of freedom are higher than the total DOF of the parameters [28].

S/N Ratio and ANOVA.
In this investigation, Minitab 18 is implemented to examine each control factor's data, and it is evaluated for the mean and S/N ratios [29][30][31]. All the belongings, on average responses, are symbolized as signals.
Computing of deviations is executed by noises from the investigational output. Based on the necessity of elevated strength for the weld joint in this research, the S/N ratio is set as "larger is better" to maximize the output, and the equation evaluating it is where y is denoting the experiential data and n is termed as the number of trials. e effects of all the TIG welding parameters of the response (tensile strength, impact strength, and hardness) are identified through statistical methods [32][33][34]. Each factor's percentage contribution is based on the exact level of confidence, and ANOVA results clearly show the responses' output.

Experiments
e TIG welding process parameters were selected based on the existing research and the trial experiments conducted for this purpose. e preferred process parameters and their levels are presented in Table 3. e AC power supply type, Keppi make, 350 W capacity TIG welding machine were employed for welding these aluminium workpieces.
e nonconsumable tungsten electrode of 3.2 mm diameter and multicomponent flux AF305 were employed in TIG welding. Constant-current flows of 55 A-15 ± 2 V, 60 A-20 ± 2 V, and 65 A-25 ± 2 V were utilized to produce arc between AA8006 aluminium alloy plates (work) and electrode in presence of pure argon as shielding gas. e gas flows over the nozzle (0.125 m dia); nozzle travel speeds of the 0.14 m/min, 0.15 m/min, and 0.16 m/min were set for experimentation.
e arc length was maintained as 0.025 meter long as constant process parameters. Protection of the welding area and the tungsten electrode are achieved by supplying inert gas. e temperature of arc produced in TIG welding process reaches up to 20,000°C; hence, it is enough to melt aluminium AA8006 metal edges and form the sound weld [35][36][37]. e welded area can be allowed to solidify for the conversion of the liquid pool into solid nature. Figure 1 illustrates the TIG-welded aluminium alloy 8006 plates effectively.

Tensile Strength of TIG-Welded AA8006 Plates.
In specimens prepared for tensile test and tested as per ASTM standard ASTM B557-06, the prepared samples and tested specimens are exhibited in Figures 2(a) and 2(b), respectively-the Universal Testing Machine (UTM) under the capacity of 400 kN employed in this investigation. e tensile strengths of the weld on AA8006 plates at various TIG-welding process parameters are presented in Table 4.

Impact Strength of TIG-Welded AA8006 Plates.
During the material's failure, the energy is observed through the impact test identified as impact strength in specimens prepared for tensile test and tested as per ASTM standard ASTM E-23. e prepared samples and tested models are exhibited in Figures 3(a) and 3(b), respectively. All the specimens are fabricated, and the test was executed by using impact testing machine. e test method is termed the Charpy test with the range of 300 J. Figures 4(a) and 4(b) show the images of impact test specimens before and after the test were performed. e observations of impact strength of TIG-welded AA8006 plates are furnished in Table 5.

Surface Hardness of TIG-Welded AA8006 Plates.
Hardness is one of the ultimate properties of all materials; a Rockwell hardness testing machine was utilized to perform the welded zone's hardness. e intention selection was achieved based on the material such as aluminum alloy preferably 1/16″ hard steel ball applying load of 100 kgf. e test was performed in the Rockwell hardness tester; the indentation was marked on the weld bead effectively. e average readings of hardness were taken to estimate the hardness values of all specimens. Figure 5 illustrates the Rockwell hardness testing specimens effectively. e tested surface hardness of TIG-welded AA8006 plates is consolidated and presented in Table 6.            55  140  26  2  170  60  150  28  3  170  65  160  36  4  180  55  140  16  5  180  60  150  23  6  180  65  160  41  7  190  55  140  12  8  190  60  150  24  9 190 65 160 30

Advances in Materials Science and Engineering
Advances in Materials Science and Engineering

Surface Quality of TIG-Welded AA8006 Plates.
e surface quality of TIG-welded AA8006 plates is investigated. e SEM images were converted into 3D profilometric photos, and all nine images represented the tensile behavior of each specimen. e images are presented and discussed in the next section.

Results and Discussion
In this analysis, the tensile strength, impact strength, and hardness values were determined, and they estimated TIG process parameters' effect. Table 7 presents the experimental input value, response, means, and signal-to-noise ratio.

Tensile Strength.
e influence of TIG welding process parameters on the strengths of weld was statistically analyzed by using Minitab 18 software, in which the experimental data are converted into mean and S/N ratios to determine the optimal process parameters. e response for means and SN ratio values is tabulated in Tables 8 and 9, respectively.
From the analysis, the optimum parameter is determined as PC 3 BC 1 WS 1 . From Tables 8 and 9, it is inferred that the most significant parameter concerning tensile strength is base current (BC 1 -55 Amps), followed by welding speed (WS 1 -140 mm/min) and peak current (PC 3 -190 Amps). Figures 6 and 7 show the main effect plots for mean and S/N ratio: the increase of peak current increases the tensile strength, and the 190 Amps peak current offered excellent tensile strength. e 55 Amps and the 140 mm/min welding speed provided the maximum tensile strength. Figure 4 illustrates the residual plots for tensile strength. e four-in-one graph explained well the influence of factors level. e nine samples were reflected in the form of points; all the points are nearer to it; the normal probability plot points out of the maximum points are lying on the mean line since the elected model was exceptional. In the histogram plot, all the rectangular boxes are distributed regularly in a manner. In the observation order, more than 70% of points are crossed across the line; it notifies that the factor chosen was the very intellectual approach. e ANOVA is used to examine the significance of the process parameters which affect the responses. e Fisher test (F-test) is also used to investigate the importance of factors that affect the output responses. In this study, among the three elements, the base current has a higher F-value, and therefore it is considered to affect the tensile strength. Analysis of variance (ANOVA) of S/N ratio for tensile strength is presented in Table 10. Based on the ANOVA results, base current is considered the most significant parameter (67.66%), which affects the tensile strength followed by welding speed and peak current. Welding speed contributes 38.08% and peaks current 0.19%.  Figure 8(c) demonstrates the 140 mm/min welding speed, and 190 Amps of the peak current induced the maximum tensile strength.

Impact Strength.
Using Minitab, all the investigational data are altered into mean and S/N ratios to estimate the optimum process parameters. In this study, the effect of process parameters and levels is determined as PC 1 BC 3 WS 1 and tabulated the means and SN ratio values in Tables 11 and 12, respectively.             Advances in Materials Science and Engineering Figure 11 illustrates the residual plots for impact strength, from the four-in-one graph elucidated fine for influencing factors level. All nine samples were tested, and the results were reflected in the form of graphical representation. In this plot, all the points are closer to it; the normal probability plot noticed the maximum issues lying on the mean line since the designated model was incomparable. From the histogram plot, all the rectangular boxes are distributed as standard in mode.
e Fisher test (F-test) is used to study which factors affect the output responses. In this work, among the three parameters, base current has a higher F-value, and therefore, it is considered to have effects on the impact strength. Analysis of variance (ANOVA) of S/N ratio for impact strength is presented in Table 13. e base current is considered the most significant parameter (71.63%) from the ANOVA outcome, affecting the impact strength followed by peak current 14.69% and welding speed 10.20%. Figures 12(a)-12(c) show the contour plot of impact strength directly influencing two parameters. e maximum impact strength is obtained by the interaction of high base current and low peak current, high base current and low welding speed, and low welding speed and peak current.

Hardness Test.
From the hardness test, the input parameters rank and its effects are studied through Minitab, and all the investigational data are translated into mean and S/N ratios value. e response for means and SN ratio values are tabulated in Tables 14 and 15, respectively. e tables visibly identified the key parameters in this study. e base current has highly influenced this analysis, followed by peak current and welding speed based on the delta value and rank order. e hardness test's optimal parameters were obtained as peak current of 190 Amps, the base current of 55 Amps, and welding speed of 160 mm/min. Figures 13 and 14 show the main effect plot for mean and main effect plot for S/N ratio, respectively. e increasing peak current increases the hardness value; applying 190 Amps provided the maximum hardness value. e minimum base current of 55 Amps offered the maximum hardness value; increasing base current reduces the hardness value. Increasing the welding speed from 140 mm/min to 160 mm/min would increase the hardness value. Figure 15 presents the residual plots for hardness test; this four-in-one graph enlightens the parameters influencing it in different form. Each sample input and output value were tested and obtained; the results were replicated in the graph. From this plot, all the points are very close to the mean line. It would be noted in the probability plot versus fit graph. In the histogram plot, all the rectangular boxes' values are distributed evenly in the standard one.
From the ANOVA, significant parameter values are analyzed through the Fisher test (F-test); F-test was also used to inspect the influential factors which affect the output responses. From this study, among three aspects, the base current has a higher F-value. erefore, it is considered to be an affecting factor of the hardness. Analysis of variance of S/ N ratio for hardness test is presented in Table 16. e base current is highly contributed from the ANOVA results, such as 76.01%, which affect the hardness followed by the peak current 11.24%, and welding speed contributes 9.11%. e P value of the base current was 0.001; it was within the limit of 0.005. Figure 16(a) illustrates the contour plot of hardness vs. peak current and base current; the maximum hardness was obtained as the involvement of peak current of 190 Amps and the base current of above 55 Amps. e lowest peak current value and the highest base current value offered minimum hardness value. Figure 16(b) quickly found out the minimum and maximum hardness value, the low base current, and high welding speed as 160 mm/min           conversion of SEM images into 3D profilometric images. All nine images represented the tensile behavior of each specimen. In Figure 17, each image is filled with two different colours like pink and green. Where the pink colour is noticed, the welded area possesses high denser material formation to avoid the material's tensile failure and also demonstrates the welding strength [38]. e green colour indicated the place of the weaker section of the material at which the material weld has low density and low tensile strength. According to this, in Figures 17(a) and 17(d), samples were welded strongly more than the other 7 samples. Hence the dense pack of weld material could be achieved by means of input parameters utilized for first and fourth sample welding. Advances in Materials Science and Engineering

Conclusions
e experimental investigation of AA8006 TIG welding was carried out fruitfully. Mechanical properties such as Rockwell hardness, impact strength, and tensile strength were estimated with influence of chosen parameters, and the result of this investigation was concluded as follows: (i) e optimum parameter is determined from the tensile test analysis as PC 3 BC 1 WS 1 , and the optimal values are base current 55 Amps, followed by welding speed 140 mm/min and peak current 190 Amps. From the ANOVA results, the base current is considered the most significant parameter, and its contribution is 67.66%, further followed by welding speed and peak current of 38.08% and 0.19%, respectively. (ii) In the impact strength, the optimal parameters were attained as PC 1 BC 3 WS 1 , and its values were peak current of 170 Amps, base current of 65 Amps, and the welding speed of 140 mm/min. From the ANOVA conclusion, the base current is considered the most significant parameter. Its contribution is 71.63%, which affects the impact next, followed by a peak current of 14.69% and finally welding speed of 10.20%. (iii) In this study, the effect of process parameters and optimal values was determined as PC 3 BC 1 WS 3 . e result of optimal values is the peak current of 190 Amps, the base current of 55 Amps, and a welding speed of 160 mm/min. e base current is highly contributed in the ANOVA results, such as 76.01%, followed by peak current contributed as 11.24% and welding speed 9.11%. (iv) In all tests, the base current has a prime factor in the tensile, impact, and hardness test.

Data Availability
e data used to support the findings of this study are included within the article.